IJACSA Special Issue on Selected Papers from International Conference & Workshop On Advance Computing 2013 GaAs, InP, InGaAs, GaInP, p+-i-n+ Multiplication measurements for Modeling of Semiconductor as photo detectors

Sanjay.C.Patil B.K.Mishra (Research Scholar at NMIMS MUMBAI) Thakur College of Engineering and Technology, Parshvanath College of Engineering, THANE (W), Kandivali (E) Mumbai, 400101 India Mumbai, 400601 India

Abstract—Optoelectronic is one of the thrust areas for the Group III on the periodic chart (arsenic in the case of GaAs) recent research activity. One of the key components of the and one from Group V (gallium in the case of GaAs). Other optoelectronic family is photo detector to be widely used in three-five (or III-V in Roman numerals) semiconductors broadband communication, optical computing, optical include indium phosphide and gallium nitride. transformer, optical control etc. Present paper includes the investigation. carried on the basis of the. Multiplication The band gap energy of semiconductors tends to decrease measurements on GaAs, InP, InGaAs, GaInP, p+-i-n+s with – with increasing temperature. When temperature increases, the region thicknesses, with investigation of applicability of the local amplitude of atomic vibrations increase, leading too larger ionization theory. A local ionization coefficient to be increasingly inters atomic spacing. In a regular semiconductor crystal, the unrepresentative of the position dependent values in the device as band gap is fixed owing to continuous energy states. In a is reduced below 1 um. quantum dot crystal, the band gap is size dependent and can be altered to produce a range of energies between the valence Keywords— Photo detectors; Impact ionization. band and conduction band. It is also known as quantum confinement effect. I. INTRODUCTION With the advent of broadband communication, Band gaps also depend on pressure. Band gaps can be INTERNET communication, optical computing, the research either direct or indirect, depending on the electronic band in the optical devices has emerged as on of the thrust area for structure. the active and consistent research. One of such primary Gallium arsenide (GaAs) devices is the photo detector. Therefore, recent years have A compound of the elements gallium and arsenic it is an seen tremendous research activities in the area of photo III/V semiconductor, and is used in the manufacture of devices detector mathematical modeling and simulation. It includes the such as microwave frequency integrated circuits, monolithic domain like optical control of r.f./microwave devices, microwave integrated circuits, infrared light-emitting diodes, broadband communication like optical communication, as a laser diodes, solar cells, and optical windows. optoelectronic component to support green technology, etc. Indium phosphide (InP) Basic objective of the active research includes the A binary semiconductor composed of indium and reduction in the device dimension , reduction in power phosphorus. It has a face-centered cubic crystal structure, utilization, better performance against noise, ease of identical to that of GaAs and most of the III-V semiconductors integration to make complete system on chip, better reliability InP is used in high-power and high frequency electronics against all possible adverse condition and so on. At present the because of its superior electron velocity with respect to the commercially available photo detectors for the various more common semiconductors silicon and gallium arsenide. It includes PIN diode, APD, photo transistor and the recent also has a direct bandgap, making it useful for optoelectronics device like PIN FET.A photo detector operates by converting devices like laser diodes. light signals that hit the junction to a voltage or current. The junction uses an illumination window with an anti-reflect Indium gallium arsenide (InGaAs) coating to absorb the light photons. The result of the Indium gallium arsenide (InGaAs) is a semiconductor absorption of photons is the creation of electron-hole pairs in composed of indium, gallium and arsenic. It is used in high- the depletion region. Impact Ionization is the process in a power and high-frequency electronics because of its superior material by which one energetic charge carrier can lose energy electron velocity with respect to the more common by the creation of other charge carriers. For example, in semiconductors silicon and gallium arsenide. InGaAs band semiconductors, an electron (or hole) with enough kinetic gap also makes it the detector material of choice in optical energy can knock a bound electron out of its bound state (in fiber communication at 1300 and 1550 nm. Gallium indium the valence band) and promote it to a state in the conduction arsenide (GaInAs) is an alternative name for InGaAs. band, creating an electron-hole pair Three-five materials refer Gallium indium Phosphide (GaInP) to compound semiconductors made from one element from

34 | P a g e www.ijacsa.thesai.org IJACSA Special Issue on Selected Papers from International Conference & Workshop On Advance Computing 2013

GaInP, a wide band gap semiconductor lattice matched to and from photo multiplication measurements performed GaAs, is of interest for a variety of device applications such as with carrier injection from the depletion region edges. [7]-[8] heterojunction bipolar transistors (HBTs) And heterojunction field-effect transistors (HFETs) The advantages of GaInP over For electron multiplication, M e xo =0 and for pure hole GaAlAs for GaAs-based HBT applications include its large multiplication M , x =W. However, carriers entering the energy band gap (1.9 eV), lower conduction band offset, h o reduced deep-level concentration, and easier selective etching. high field region with energy much less than the ionization

GaInP-emitter HBTs with high current gain and good threshold must traverse a dead space, distance d e , for microwave performance have been reported electrons or d h for holes, before they acquire sufficient energy II. THEORY to impact ionize. With estimation this dead space distance is To design structures for high-voltage or high-power given by equating it to the ballistic distance a carrier requires applications, an accurate knowledge of impact ionization to reach the ionization threshold energy, coefficients in GaInP is necessary for calculating breakdown characteristics of junctions. In the work reported here, Eth i.e. d Eth / qF . photocurrent multiplication was used to measure the electron and hole ionization coefficients in ~100 GaInP by illuminating For a device where electrons are injected at x 0, these corrections usually disallow electron ionization in a dead- p n n diode structures from either side with above space region from 0 x d and hole ionization in the band gap radiation.6 The results show that GaInP has e significantly lower values of a and b than those of GaAs or region fromW dh x W . Okuto and Crowell [9] InP, a promising indication for high-voltage applications. presented an approximate expression relating multiplication to the ionization coefficients while accounting for the reduced multiplication by these regions. Bulmanet al[10]. simplified their expression to interpret the measured multiplication results from p -n-n junctions by assuming no electron-initiated ionization occurs within a distance from their injection point.

Physics of Impact Ionization Avalanche photo detectors (APDs) use the impact ionization principle to detect and amplify very low light signals and they are still used as the most sensitive detector for most systems. It is found that to have a high-gain, low-noise APD, the ionization rate for electrons and holes needs to be Figure.1. diode layer structure very different. Efforts to find the best material to perform impact ionization reveal that silicon has the largest ionization rate difference between electrons and holes among all semiconductors. Due to its cut-off wavelength around 1 μm, however, silicon has rarely been employed for today’s optical Fig.1. Basic structure of photo detector communication systems that use 1.55 μm wavelengths light. Suitable materials using combinations of binary and Accurate determination of the electron and hole ionization ternary/quaternary III-V semiconductors such as InGaAs on coefficients, and respectively, is important, since these are InP substrates have provided solutions for longer wavelength used to determine avalanche multiplication characteristics and detection. breakdown. Conventionally and are assumed to depend only on the local electric field, and the mean multiplication Impact Ionization Gain Mechanism due to an electron-hole pair generated at position is given by The impact ionization gain mechanism can be demonstrated by using a thermally generated electron, or an W electron created by an absorbed photon, travelling inside a exp dx semiconductor where a depletion region is formed. Figure 6 x0 M x0 illustrates the impact ionization process in a reverse biased W x 1 exp dxdx PIN. As shown in the figure, electrons can gain sufficient 0 0 kinetic energy while travelling in a high electric field. If the electric field is high enough, this high-energy electron may As described by Stillman and Wolffe [7] where W is the initiate the electron-electron scattering so that an electron in total depletion width. The electric field exists between x=0 and the valence band can be excited to the conduction band. As a x=W causing electrons to move from left to right. This result of this, another electron-hole pair is produced by expression is also traditionally used to derive the values of, promoting an electron from the valence band into the conduction band. Due to the strong electric field, the subsequent electron and hole will continue to collide with the

35 | P a g e www.ijacsa.thesai.org IJACSA Special Issue on Selected Papers from International Conference & Workshop On Advance Computing 2013 lattice and create more electron-hole pairs. Therefore, asymmetric to some degree for electrons and holes. For numerous carriers are generated and the result is a multiplied example, the ionization rate for electrons is about 5 times current output. This phenomenon is sometimes referred to as greater than holes in Germanium. For silicon, however, the avalanche breakdown electrons can ionize 50 times to 1000 times more readily than holes depending on the electric field amplitude. The Ionization Threshold Energy probability for initiating impact ionization is quantified as the The minimum energy required to excite an electron, impact ionization coefficient. It is defined as the reciprocal of however, is more than just freeing an electron from the the average distance travelled by an electron or hole to valence band. In order to decide the ionization threshold 1 energy, various methods including from the valence to the produce an electron-hole pair. Therefore, its unit is cm . For conduction band is equal to the band gap energy of the electrons, the coefficient is denoted as α. For holes, it is semiconductor. Impact ionization parabolic, non parabolic, denoted as β. Materials with very different value for α and β, realistic, and non local pseudo potential band structure have such as in silicon can create less impact ionization noise been utilized. It is found that the threshold energy differs for because only one type of carrier is dominant during the most semiconductors. It is a function of the band structure, ionization process. First, the length of the semiconductor is effective mass ratio between electron and hole, density of long (L >1 μm) such that non-local theories [4] are not state, phonon interaction, and spin-orbit splitting energy. considered. Secondly, the current density is low to avoid the space charge effect which may screen the electric field and The best way to estimate the ionization threshold energy lower the gain. A differential equation can be used to describe involves a simple two parabolic band model. In this model, we the multiplication process in terms of ionization rates α and β. consider one conduction band with effective mass me and If β is much smaller than α, (4) can be rewritten as 1 exp L one valence band with mass mh . As shown in Fig. 6, prior to M n L exp L the collision, the electron travelling from the left-hand side has 1 exp x 0 a kinetic energy of 1/2 2 and a momentum of , mevi mevi (4) where vi is the initial velocity of the electron. After collision, 1 expL three carriers exist: a new electron-hole pair plus the original M p L exp L 1 exp x electron. Electrons continue travelling to the right and the hole 0 to the left. (5) Assuming that the collision is elastic, the conservation of exp(L) energy and momentum must be satisfied these two M n assumptions are summarized as 1 exp(L) 1 2 1 2 1 2 (6) mevt Eg meve 2 mhvh A positive feedback factor (β/α) in (6) shows the effect of 2 2 2 ionization coefficients on multiplication gain. As β gets (1) bigger, but still much smaller than α, M can reaches And n breakdown in a shorter distance. m v m v m v e t e i h h If we consider an extreme case, β = 0, (2.6) can be further (2) simplified to Where Eg is the energy band gap of the semiconductor, L v is the electron velocity, and v is the hole velocity after M exp dx exp L e h n 0 the collision. Note that when m m and v v v , (1) e h e h i (7) and (2) can be derive that the required initial electron energy for ionization process as From (7) we observe that when β = 0, there is no avalanche breakdown because just continues to increase 1 2 exponentially withL . A plot is given in Fig.2 using (6) to Ei mevi 1.5Eg 2 demonstrate the gain versus L for various value of (α/β) (3) This is the well-known 3/2-band-gap rule for ionization Impact Ionization Coefficient Measurement threshold energy in semiconductor [1]. We know that α and β are strong function of electric field in the multiplication region. Electric field, however, also Ionization Coefficients and Gain Equations depends on the bias voltage, doping profile, and the device To derive the gain equations for impact ionization process, geometry. In this section, we will explain how to measure the we need to first define the impact ionization coefficient. For ionization coefficients accurately for different device most semiconductor materials, the impact ionization process is structures including p-i-n diodes.

36 | P a g e www.ijacsa.thesai.org IJACSA Special Issue on Selected Papers from International Conference & Workshop On Advance Computing 2013

In measurement, a very high energy light is used to initially injected electron. The output current decreases to zero illuminate the diode. Due to the high energy of the photons, as all the ionized holes arrive at the negatively biased electron-hole pairs can be created very close to the surface to electrode. Thus, the current pulse lasts about twice as long as obtain the pure electron or hole injection condition. Electron the transit time. Since the pulse width is independent of the ionization is measured by shining light from the p+ side. multiplication gain, there is no gain-bandwidth product Photon-excited electrons are injected into the intrinsic layer limitation when β or α = 0. while holes are swept to the left. Hole ionization is measured by illuminating light from the n+ side, injecting holes into the It is found that the avalanche multiplication process does intrinsic layer. not affect the device bandwidth as long as the dc multiplication gain M is less than α/β. On the other hand, if M The electron gain M can be calculated by dividing the > α/β, the multiplication gain becomes a function of frequency n and is expressed as total current measured for a given electric field by the photocurrent created by the light. The photocurrent can be 1 2 2 2 precisely measured when the diode is operated without 2 M() M 0 /( M 0 1 ) avalanche gain. The hole gain M p can be obtained through (10) the same process Where τ1 is an effective transit time and is approximately τ1 = N(β/α)τ. N is a number varying slowly from 1/3 to 2 as β/α varying from 1 to 103 , and τ is the transit time equal to

L / vs where L is the length of the avalanche gain region and

vs is the saturation velocity

The gain-bandwidth product for M > α/β can be obtained using (10) for high frequencies and is expressed as

M 1 1 0 M () 1 2 2 2 1 N( ) ( M 01 ) (11)

Equation (11) indicates the basic requirements for an impact-ionization based device to obtain a high gain- Fig.2. Multiplication gain M versus αL for pure electron injection. bandwidth product. These requirements include a small β/α Various α/β value are used to demonstrate its effect on avalanche breakdown value and short intrinsic time. Therefore, a correct choice of curve material, multiplication layer thickness, and carrier transport velocity are essential. . Once and M p are known, we can use equation (4) Using (10), the calculated frequency response for a P-I-N and (5) to derive formulas related α and β to and . structure with 1m thick gain region when operating at They are calculated to be M=50 is given in Figure 3. Using Matlab to simulate the both the measure of α and β since Bulmanet al [10]. found that β > α, these two sets of 1 M n 1 M n ln parameters for the coefficients since they enable the data to be L M M M n p p more accurately quantified over the wide field range the (8) coefficients are parameterized in The impact ionization And coefficients can be fitted into an exponential form:

1 M p 1 M p ln (9) (E) A exp(B / E) e e L M p M n M n (E) Ah exp(Bh / E)

CeH Impact Ionization Response eH AeH exp[(Beh /) The carrier build-up time in the multiplication process Aexp[(B /)C depends on the contribution of carrier feedback In the ideal h For the local calculation the values of α and β were taken condition, where only one type of carrier is capable of from.[10] for electric fields, F, This investigation involved initiating impact ionization process (electrons for β = 0), the measuring both the multiplication and excess noise output current pulse increases with the transit time for the

37 | P a g e www.ijacsa.thesai.org IJACSA Special Issue on Selected Papers from International Conference & Workshop On Advance Computing 2013 characteristics of several samples with overlapping field CeH eH AeH exp[(Beh /) regions and represents the most extensive and rigorous to date C Impact Ionisation coefficient and Multiplication of h Aexp[(B /) electrons & holes for GaAs Impact Ionisation Coefficients for InGaAs (narrowband Impact Ionisation Coefficients for GaAs gap semiconductor) great importance in the case of an 7 7 1.82 1 ionization coefficient which increases with temperature that (E) 1.8910 [(exp((5.7510 )/ E) ]cm can result in an unstable positive power dissipation feedback (E) 2.21107[(exp((6.57 107 )/ E)1.75]cm 1 which the voltage breakdown can be obtained by extrapolating the multiplication curveAs shown in fig 6

For alpha

Fig.3. Frequency Response of a P-I-N photodiode with 1m thick multiplication layer. Notice that parameter k is define as β/α Fig.5. simulated of multiplication w 0.48m device as a function Multiplication of electrons and holes for GaAs Simulation of calculate Electron and hole multiplication of temperature from 20K to 500K factors for a range of ideal p-i-n s with from 1 um down to 4 2 1 0.48um for GaAs with temperatures of 20K to 500K, Shown AeH 7.2597 10 (24.204T) (0.3259T )cm in figure 5 increasing temperature causes the multiplication of 5 2 2 electrons and holes to shift to higher voltage therefore higher BeH 5.998810 (3.476310 T) (2.4768T )V / cm electric fields are required to offset the increase in carrier C 1.783 (7.2548104 T) cooling by phonon scattering and maintain multiplication eH For beta

A 6.1026105 (9.6637 102 T) (1.1384T 2 )cm 1 6 3 2 B 1.339410 (1.069910 T) (20.4507T )V / cm C 1.0910 (2.3505104 T)

Fig.4. Impact Ionisation Coefficients for GaAs versus inverses electric field

Impact Ionisation coefficient and Multiplication of Fig.6. Impact Ionisation Coefficients for InGaAs versus inverses electric electrons & holes for InGaAs field Multiplication of electrons and holes for InGaAs

38 | P a g e www.ijacsa.thesai.org IJACSA Special Issue on Selected Papers from International Conference & Workshop On Advance Computing 2013

Simulation of Electron multiplication factors that depends (E) 1.62106[exp((2.11106 )/ E]cm 1 on temperature with the thickness of 1.3um and 1.9 um for InGAas p-i-ns from 20K to 400K and hole multiplication with thickness of 3.0um as n-i-p from 20K-300K. The results from figure 7 show a very limited increase in photocurrent initially and then the sudden and clear onset of the avalanche multiplication process. T

Fig.8. Impact Ionisation Coefficients for InP versus inverses electric field

Multiplication of electrons and holes for InP The results from figure 9 show that the temperature dependence of multiplication is not uniform, since the multiplication curves with thickness of the materials from 0.24 to 2.40um respectively. Simulation of Electron multiplication factors for a range of ideal p-i-ns with from 0.24um down to Fig.7. Simulated of multiplication characteristics of 1.3 and 1.9 um thick 2.40um for InP with temperatures of 20K to 500K InGaAs p-i-n diode from 20–400 K As a test of the parameterized coefficients, test shows for all the materials, the predicted multiplication for an ideal Impact Ionisation coefficient and Multiplication of diode, compared with the measured characteristic. It can be electrons & holes for InP seen that the agreement is good, both at low and high The electron and hole ionization coefficients can be multiplications using matlab for these simulations for extracted from the measured multiplication results if both wideband gap semiconductor and narrowband gap electrons initiated and hole initiated multiplication results are semiconductor. available for the same structure When an electron (or hole) initiates themultiplication process, an electric current is The structures for high-voltage or high-power applications, induced by the moving electronsand holes within the an accurate knowledge of impact ionization coefficients in multiplication region GaInP is necessary for calculating breakdown characteristics of junctions. InP has high electron peak velocities resulting from large inter valley separation and good breakdown properties owed to In the work reported here, photocurrent multiplication was a relatively low electron impact ionization coefficient used to measure the electron and hole ionization coefficients from either side with above bandgap radiation. Compared to the data of GaAs and InP illustrated in Fig.6 and Fig. 8, GaInP has the lowest values of α and β, signifying The results show that GaInP has significantly lower values a higher breakdown voltage. Moreover, the slopes of the of α and β than those of GaAs or InP, a promising indication curves of α and β vs 1/E for GaInP shown in Fig. 7 are steeper for high-voltage applications. than for the others.

Impact Ionisation Coefficients for InP

(E) 2.93106[exp((2.64106 )/ E]cm 1

39 | P a g e www.ijacsa.thesai.org IJACSA Special Issue on Selected Papers from International Conference & Workshop On Advance Computing 2013

Simulation of Electron multiplication factors for a range of ideal p-i-n s with from 0.24um down to 2.40um for GaInP with temperatures of 300K

Fig.9. Simulated of multiplication characteristics of 0.24 and 2.40 um thick for InP p-i-n diode from 20–400 K

Impact Ionisation coefficient and Multiplication of electrons & holes for Fig.11. Simulated of multiplication characteristics of 0.24 um thick for GaInP GaInP p-i-n diode from 300 K Impact Ionisation Coefficients for GaInP(wideband gap semiconductor) 6 6 1 (E) 3.8510 [exp((3.17 10 )/ E]cm III. RESULT AND DISCUSSION 6 6 1 (E) 1.7110 [exp((3.1910 )/ E]cm Voltage breakdown due to avalanche multiplication, also The electron and hole multiplication factors, Mn and Mp, defined as the reverse bias voltage where multiplication rate are defined as the total output photocurrent divided by the goes to infinity naturally of great practical interest. electron or hole current injected at the contacts. Results for The voltage VB is defined as the reverse-bias voltage Mn and Mp from respective measurements are shown in Fig across the multiplication region at which the mean gain 10. becomes infinite. In these results, slight corrections were made to the In doing so rather then testing with hands on materials in injected currents due to slightly voltage-dependent intrinsic fab or clean room physically testing the materials, with this reverse currents. Because the widths of the depletion regions simulation we can create a model and simulate any materials depend on bias, the number of thermally generated minority first with respect to their voltage breakdown versus thickness carriers that diffuse into the depleted n region also varies. (width) without wasting unnecessary time and cost for testing This leads to a slight increase of the injected current as the of materials reverse bias is increased Case 1 GaAs wide band gap, highly resistive which makes it a very good electrical substrate therefore makes it a very good material for ideal material for microwave and millimeter wave integrated circuits. It can also be operated at higher power levels because they have higher breakdown voltage.

Fig.10. Impact Ionisation Coefficients for GaInP versus inverses electric field

Multiplication of electrons and holes for GAInP

40 | P a g e www.ijacsa.thesai.org IJACSA Special Issue on Selected Papers from International Conference & Workshop On Advance Computing 2013

Fig.12. Simulated of voltage breakdown versus thickness for GaAs

Case 2 GaInP wideband gap semiconductor exhibits high breakdown voltage characteristics indicating that it is a good choice of material for high power applications. This suggests that the ideal electric field distribution assumption is valid and that edge effects are not important in this material system for mesa geometry structures. Note that since these punches through devices have a low carrier concentration in the n region and high breakdown voltage, the effects of dead space could be ignored. And data were used to calculate the expected breakdown voltages for p-i-n diode with various thicknesses

Fig.13. Simulated of voltage breakdown versus thickness for InP

InP wideband gap have an advantage compared to GaAs for many applications when used in high-field regions of the device profile, can significantly improve device performance. These applications include high performance power amplifier for cellular phones, ultra-efficient ultra-linear power amplifiers ideally suited for digital communication systems and satellite networks ICs, and highly integrated mixed signal and high-speed fiber-optic circuits. Wide bandgap semiconductors are associated with a high breakdown voltage. This is due to a larger electric field required to generate carriers through impact mechanism. Case 4

Fig.12. Simulated of voltage breakdown versus thickness for GaInP

GaInP wideband gap semiconductor exhibits high breakdown voltage characteristics indicating that it is a good choice of material for high power applications. This suggests that the ideal electric field distribution assumption is valid and that edge effects are not important in this material system for mesa geometry structures. Note that since these punches through devices have a low carrier concentration in the region and high breakdown voltage, the effects of dead space could be ignored. And data were used to calculate the expected breakdown voltages for p-i-n diode with various thicknesses Fig.14. Simulated of voltage breakdown versus thickness for InGaAs Case 3 InGaAs with narrow band gap is also a popular material in infrared detectors and some short wave infrared cameras. It also has lower multiplication noise than germanium when used as the active multiplication layer of an avalanche photodiode. Also has a low breakdown voltage

IV. CONCLUSION For this research work materials are simulated base on p-i- n diodes therefore very little studies on Avalanche Photodiode (APD) and Schottky Barrier diodes. The carriers are absorbed in a π- region. The absorption leads to the generation of electron-hole pairs in this region.

41 | P a g e www.ijacsa.thesai.org IJACSA Special Issue on Selected Papers from International Conference & Workshop On Advance Computing 2013

The electric field in the π-region is high enough to separate the [12] M. M. Hayat, B. E. A. Saleh, and M. C. Teich, “Effect of dead space on carriers. The electric field across the π-region is not high gain and noise of double-carrier-multiplication avalanche photodiodes,” IEEE Trans. Electron Devices, vol. 39, pp. 546–552, Mar. 1992. enough for the charge carriers to gain enough energy for [13] M. M. Hayat, W. L. Sargeant, and B. E. A. Saleh, “Effect of dead space multiplication to take place. on gain and noise in Si and GaAs avalanche photodiodes,” IEEE J. Quantum Electron, vol. 28, pp. 1360–1365, May 1992. REFERENCES [14] A. Di Carlo and P. Lugli, “Dead-space effects under near breakdown [1] [1] B.K.Mishra,computerAidedmodelingof solidstate photodetectors conditions in AlGaAs/GaAs HBT's,” IEEE Electron Device Lett., vol. Ph.DthesisBirlainstituteoftechnology,Mesra,Ranchi 1995 14, pp. 103–105, Mar. 1993. [2] T. P. Pearsall, “Impact ionization rates for electrons and holes in [15] S. P. Wilson, S. Brand, and R. A. Abram, “Avalanche multiplication Ga0.47In 0.53As,” Appl. Phys. Lett. 36, 218-220 (1980) properties of GaAs calculated from spatially transient ionization [3] S. Wang, R. Sidhu, X. G. Zheng, X. Li, X. Sun, A. L. Holmes, Jr., and J. coefficients,” Solid-State Electron., vol. 38, pp. 2095–2100, Nov. 1995. C. Campbell, IEEE Photonics Technol. Lett. 13, 1346 (2001). [16] A. Di Carlo and P. Lugli, “Dead-space effects under near breakdown [4] B.K.Mishra, LochanJolly, S.C.Patil,” In Ga As a next generation 1-x x conditions in AlGaAs/GaAs HBT's,” IEEE Electron Device Lett., vol. material for photodetectors “,JSAM.2011 14, pp. 103–105, Mar. 1993. [5] R.Poerschke,Shpringer–Verlag,Madelung,O.(ed.),Semiconductor: group [17] S. P. Wilson, S. Brand, and R. A. Abram, “Avalanche multiplication IV elements and III-V compound. Series "Data in science and properties of GaAs calculated from spatially transient ionization technology, Berlin, 164 (1991). coefficients,” Solid-State Electron., vol. 38, pp. 2095–2100, Nov. 1995. [6] J. R. Chelikowsky, and M. L. Cohen, Phys. Rev. B14, 556 (1976). [18] IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 50, NO. [7] R. J. McIntyre, “A New Look at Impact Ionization – Part I: A Theory of 10, OCTOBER 2003 2027 Gain, Noise, Breakdown Probability, and Frequency Response,” IEEE [19] IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 50, NO. Trans. Electron Devices, vol. 46, 1623—1631 (1999). 10, OCTOBER 2003 2021 Temperature Dependence of Breakdown and [8] H. Ando and H. Kanbe, “Ionization coefficient measurement in GaAs by Avalanche Multiplication in In0:53Ga0:47As Diodes and Heterojunction using multiplication noise characteristics,” Solid-State Electron., Bipolar Transistors M. Yee, W. K. Ng, J.P. R. David, Senior Member, vol. 24pp. 629–634, 1981. IEEE, P. A. Houston, C. H. Tan, and A. Krysa [9] O.Konstantinov, Q.Wahab, N. Nordell, and U. Lindefelt, “Ionization [20] Shanghai Institute of Technical Physics Theory Study of SAGCM InP rates and critical fields in 4H silicon carbide,” Appl. Phys. Lett., vol. 71, L. Lin, W. J. Wang, N. Li, X. S. Chen and W. Lu Shanghai Institute of July 1997 Technical Physics, Chinese Academy of Sciences National Lab for [10] Y.Okuto and C. R. Crowell, “Ionization coefficients in semiconductors,” Infrared Physics, Phys. Rev. B., vol. 10, pp. 4284–4296, Nov. 1973. [21] Impact ionization coefficients in (100) GaInP S.-L. Fu, T. P. Chin, M. C. [11] G. E. Bulman, V. M. Robbins, and G. E. Stillman, “The determination Ho, C. W. Tu, and P. M. Asbeck Department of Electrical and Computer of impact ionization coefficients in (100) gallium aresenide using Engineering, University of California, San Diego, La Jolla, California avalanche noise and photocurrent multiplication measurements,” IEEE 92093 Trans. Electron Devices, vol. ED-32, pp. 2454–2466, Nov. 1985.

42 | P a g e www.ijacsa.thesai.org